title: Nickel–zinc battery
text: A nickel–zinc battery, abbreviated NiZn, is a type of rechargeable battery similar to NiCd batteries, but with a higher voltage of 1.6 V.
  
  Larger nickel–zinc battery systems have been known for over 100 years. Since 2000, development of a stabilized zinc electrode system has made this technology viable and competitive with other commercially available rechargeable battery systems. Unlike some other technologies, trickle charging is not recommended.
  
  History 
  In 1901 Thomas Alva Edison was awarded  for a rechargeable nickel–zinc battery system.
  
  The battery was later developed by the Irish chemist Dr. James J. Drumm (1897–1974), and installed in four two-car Drumm railcar sets between 1932 and 1949 for use on the Dublin–Bray railway line. Although successful, they were withdrawn when the batteries wore out. Early nickel–zinc batteries provided only a small number of discharge/recharge cycles. In the 1960s nickel–zinc batteries were investigated as an alternative to silver–zinc batteries for military applications, and in the 1970s were again of interest for electric vehicles. Evercel Inc. developed and patented several improvements in nickel–zinc batteries, but withdrew from that area in 2004.
  
  Applications 
  Nickel–zinc batteries have a charge/discharge curve similar to 1.2 V NiCd or NiMH cells, but with a higher 1.6 V nominal voltage.
  
  Nickel–zinc batteries perform well in high-drain applications, and may have the potential to replace lead–acid batteries because of their higher energy-to-mass ratio and higher power-to-mass ratio — as little as 25% of the mass for the same power. NiZn are cheaper than nickel-cadmium batteries, and are expected to be priced somewhere between NiCd and lead–acid types. NiZn may be used as a substitute for nickel–cadmium. The European Parliament has supported bans on cadmium-based batteries; nickel–zinc is a good alternative for power tools and other applications. A disadvantage is increased self-discharge rate after about 30-50 cycles, so that batteries do not hold their charge as long as when new. Where this is not a problem NiZn is a good battery choice for applications requiring high-power and high-voltage.
  
  Battery life 
  Compared with cadmium hydroxide, the tendency of the soluble zinc hydroxide ion (zincate) to dissolve into solution and not fully migrate back to the cathode during recharging has, in the past, presented challenges for the commercial viability of the NiZn battery. Another common issue with zinc rechargeable batteries is electrode shape change and dendrites (or "whiskers"), which may reduce the cell discharging performance or, eventually, short out the cell, resulting in a low cycle life.
  
  Recent advances have enabled this problem to be greatly reduced. These advances include improvements in electrode separator materials, inclusion of zinc material stabilizers, and electrolyte improvements (e.g. by using phosphates). PowerGenix has developed 1.6 V batteries with claimed battery cycle life comparable to NiCd batteries.
  
  Battery cycle life is most commonly specified at a discharge depth of 80 percent of rated capacity and assuming a one-hour discharge current rate. As the discharge current or the depth of discharge is reduced, the number of charge-discharge cycles for a battery increases. When comparing NiZn to other battery technologies, cycle life comparisons may vary depending on the discharge rate and depth of discharge used.
  
  Advantages 
  Nickel–zinc cells have an open circuit voltage of 1.85 volts when fully charged, and a nominal voltage of 1.65 V. This makes NiZn particularly suitable for electronic products that require the 1.5 V of alkaline primary cells rather than the 1.2 V of most rechargeable cells (most circuits tolerate the slightly higher voltage), and will not function correctly beyond, typically, the endpoint voltage of an alkaline cell. The output voltage of a 1.2 V rechargeable cell will drop to this point before it has fully delivered its charge.
  
  For use in multi-cell batteries, the higher voltage of NiZn cells requires fewer cells than NiCd and NiMH for the same voltage. They have low internal impedance (typically 5 milliohms), which allows for high battery discharge rates, up to 50C. (C is battery capacity in Ah, divided by one hour.)
  
  Newer cells which are more powerful and have a life of up to 800 cycles can be an alternative to Li-ion batteries for electric vehicles.
  
  NiZn batteries do not use mercury, lead, or cadmium, or metal hydrides, all of which can be difficult to recycle. Both nickel and zinc are commonly occurring elements in nature, and can be fully recycled. NiZn cells use no flammable active materials or organic electrolytes, and later designs use polymeric separators which reduce the dendrites problem.
  
  Properly designed NiZn cells can have very high power density and good low-temperature discharging performance, and can be discharged to almost 100% and recharged without problems.  they were available in sizes up to F, and 50Ah/ prismatic cell.
  
  Zinc is a cheap and abundant metal, the 24th most abundant element in the Earth's crust, and is not dangerous to health.
  Common oxidation is +2, so charge and discharge move two electrons instead of one as in NiMH batteries.
  
  Charging
  Chargers for NiZn batteries must be capable of charging a battery with a fully charged voltage of 1.85 V per cell, higher than the 1.4 V of NiMH. NiZn technology is well suited for fast recharge cycling, as optimum charge rates of C or C/2 are preferred.
  
  Known charging regimes include a constant current of C or C/2 to cell voltage = 1.9 V. One manufacturer recommends charging at a constant current of C/4 to C until cell voltage reaches 1.9V, then continuing to charge at a constant voltage of 1.9V until charge current declines to C/40.
  
  Maximum charge time was stated in 2009 to be about 3 hours. Once charged, continuous trickle charging is not recommended, as recombination is not provided for, and excess hydrogen will eventually vent, adversely affecting battery cycle life. Some chargers for NiZn batteries state that they do not trickle charge after the battery is fully charged, but shut off.
  
  Chemistry
  
  (−) electrode: 		 Zn + 4 OH−  Zn(OH)42− + 2e− (E0 = −1.2 V/SHE )
  
  Electrolyte: KOH
  
  Zn(OH)42−  Zn(OH)2 + 2OH−
  Zn(OH)2  ZnO + H2O
  
  (+) electrode: 	      2 NiO(OH) + 2 H2O + 2 e−   2 Ni(OH)2 + 2 OH− (E0 = +0.50 V/SHE)
  
  Overall reaction: 	   Zn + 2 NiO(OH) + H2O   ZnO + 2 Ni(OH)2
  
  Parasitic reaction: 	  Zn + 2 H2O → Zn(OH)2 + H2
  
  See also
   Comparison of battery types
   List of battery sizes
   List of battery types
   Nickel–cadmium battery
   Zinc–air battery
  
  References
  
  Nickel
  Rechargeable batteries
  Zinc